**Low temperature characterization of high efficiency **

**spin-filter Josephson junctions**

*Roberta Caruso*1,2,3,∗* _{, Halima Giovanna Ahmad}*1,2

*4,5*

_{, Avradeep Pal}*1,2*

_{, Giovanni Piero Pepe}_{,}

*Davide Massarotti*6,2

*5*

_{, Mark G. Blamire}*1,2*

_{, and Francesco Tafuri}1_{Dipartimento di Fisica E. Pancini, Università degli Studi di Napoli Federico II, Monte S. Angelo, via}

Cinthia, I-80126 Napoli, Italy

2_{CNR-SPIN, c/o Complesso di Monte S. Angelo, via Cinthia, I-80126 Napoli, Italy}
3_{SeeQC-eu, via dei Due Macelli 66, I-00187 Roma, Italy}

4_{Indian Institute of Technology Bombay, Main Gate Rd, IIT Area, Powai, Mumbai, Maharashtra}

400076, India

5_{Department of Materials Science and Metallurgy, University of Cambridge, 27 Charles Babbage Road,}

Cambridge CB3 0FS, United Kingdom

6_{Dipartimento di Ingegneria Elettrica e delle Tecnologie dell’Informazione, Università degli Studi di}

Napoli Federico II, via Claudio, I-80125 Napoli, Italy

**Abstract.** The interplay between superconducting and ferromagnetic order
pa-rameters in S/F interfaces gives rise to a wide range of peculiar properties with
applications in high-efficiency computation and in the emerging field of
super-conducting spintronics. In NbN/GdN/NbN Josephson junctions, GdN barriers
give unique properties due to the double insulting and ferromagnetic nature of
the material, as demonstrated in previous works. Here we focus on tunneling
spectroscopy of these junctions down to 0.3 K when changing the barrier
thick-ness, which contributes to complete a consistent picture on the physics of these
junctions and supports the previous indications of equal-spin Cooper pairs
con-tributing to the total supercurrent of the devices.

**1 Introduction**

In the last twenty years, the advancements in thin film deposition have made possible the
realization of superconductor/ferromagnet heterostructures, and a subsequent rich literature
on the experimental characterization and the theoretical modeling of such systems. However,
most of this literature focuses on metallic junctions, employing a wide range of ferromagnets
as weak links. Spin filter Josephson junctions are characterized by a barrier with the unique
double nature of ferromagnet and insulator. These junctions have been predicted to have a
number of interesting properties for applications in the field of low dissipation quantum and
classical computation, such as π-shifts with intrinsically low dissipation [1, 2] and
*unconven-tional temperature dependence of the critical current IC*[3]. The first realization of spin-filter
*NbN/GdN/NbN Josephson junctions, together with an unconventional IC(T) down to 4.2 K*
*has been reported in [4]. Evidences of an anomalous I(φ) compatible with triplet correlations*
have been shown in [5]. Further demonstrations of the anomalous properties of these systems

have been reported recently [6, 7]. Here we present conductance measurements confirming the previous indications of equal-spin coupling inside the barrier.

**2 Methods**

The junctions used in this work are NbN/GdN/NbN junctions with different barrier thick-nesses, ranging from 1.5 nm to 4 nm, realized during the same deposition run to ensure the same deposition conditions for all samples, using methods described elsewhere [5]. Measure-ments have been performed using an Heliox VL evaporation cryostat with base temperature of 0.3 K, with customized low noise filter detailed in [8, 9].

One of the peculiarities of the ferromagnetic junctions with insulating barriers is the spin
filtering property. The presence of an exchange field due to the ferromagnet gives rise to
two different barrier heights for spin-up and spin-down electrons. In this case, electrons
seeing a higher barrier have an exponentially lower tunneling probability, and so the current
*passing through the junction is spin-polarized. The spin-polarization P can be calculated*
*from experimental R(T) curves using the approximate relation P ≈ tanh*cosh−1σ

σ∗

, where
σis the measured conductance and σ∗_{is the conductance in absence of exchange field [4]. In}
*Fig. 1, the black dots are the measured resistance R ∝ 1/σ, while the red lines are obtained*
*by fitting experimental R(T) above TCurieand then extrapolating R*∗_{below TCurie.}

*Figure 1. R(T) curves for samples with different barrier thicknesses. Black dots are experimental*
points, red line is the resistance obtained by fitting data with a standard semiconducting model below

*TCurie*. Left: junction with low spin polarization. Right: junction with high spin polarization, the

*resistance drop below TCurie*is clearly visible.

In order to measure the conductance spectra the junctions are current biased with a sum
of two signals: a low frequency (1mHz) triangular ramp, and a small sinusoidal excitation
at about 30 Hz. The optimal ratio between the two signal amplitudes is 10−3_{. The output}
dV is read using a lock-in amplifier, while dI corresponds to the amplitude of the sinusoidal
excitation. The quasi-dc output due to the low frequency component of the bias is read using a
standard multimeter. Details of the procedure can be found elsewhere [10]. A small magnetic
field is applied to suppress the Josephson current in the junction, such field is chosen so that it
*correspond to one of the minima of the IC(H) pattern, and it is much smaller than the critical*
field of GdN, so it does not affect significantly the main features of the conductance spectra
attributed to spin filtering.

have been reported recently [6, 7]. Here we present conductance measurements confirming the previous indications of equal-spin coupling inside the barrier.

**2 Methods**

The junctions used in this work are NbN/GdN/NbN junctions with different barrier thick-nesses, ranging from 1.5 nm to 4 nm, realized during the same deposition run to ensure the same deposition conditions for all samples, using methods described elsewhere [5]. Measure-ments have been performed using an Heliox VL evaporation cryostat with base temperature of 0.3 K, with customized low noise filter detailed in [8, 9].

One of the peculiarities of the ferromagnetic junctions with insulating barriers is the spin
filtering property. The presence of an exchange field due to the ferromagnet gives rise to
two different barrier heights for spin-up and spin-down electrons. In this case, electrons
seeing a higher barrier have an exponentially lower tunneling probability, and so the current
*passing through the junction is spin-polarized. The spin-polarization P can be calculated*
*from experimental R(T) curves using the approximate relation P ≈ tanh*cosh−1σ

σ∗

, where
σis the measured conductance and σ∗_{is the conductance in absence of exchange field [4]. In}
*Fig. 1, the black dots are the measured resistance R ∝ 1/σ, while the red lines are obtained*
*by fitting experimental R(T) above TCurieand then extrapolating R*∗_{below TCurie.}

*Figure 1. R(T) curves for samples with different barrier thicknesses. Black dots are experimental*
points, red line is the resistance obtained by fitting data with a standard semiconducting model below

*TCurie*. Left: junction with low spin polarization. Right: junction with high spin polarization, the

*resistance drop below TCurie*is clearly visible.

In order to measure the conductance spectra the junctions are current biased with a sum
of two signals: a low frequency (1mHz) triangular ramp, and a small sinusoidal excitation
at about 30 Hz. The optimal ratio between the two signal amplitudes is 10−3_{. The output}
dV is read using a lock-in amplifier, while dI corresponds to the amplitude of the sinusoidal
excitation. The quasi-dc output due to the low frequency component of the bias is read using a
standard multimeter. Details of the procedure can be found elsewhere [10]. A small magnetic
field is applied to suppress the Josephson current in the junction, such field is chosen so that it
*correspond to one of the minima of the IC(H) pattern, and it is much smaller than the critical*
field of GdN, so it does not affect significantly the main features of the conductance spectra
attributed to spin filtering.

*Figure 2. Conductance spectra for junctions with P ≤ 20% (a), P ≈ 97% (e) and P ≈ 99% (i) at 0.3 K*
and at 10 K. The temperature evolution of the peak at zero bias is shown in (b), (f) and (j) respectively.
The peak height is reported on Y axis as the ratio between the zero bias peak height and the height of the
peak corresponding to the superconducting gap. Panels (d), (h) and (l) show the overlap of the positive
and negative branch of the curves at 0.3 K for the three samples mentioned above. The shift between the
two branches is proportional to the ferromagnetic exchange energy. In panels (c), (g) and (k) we show
the critical current as a function of temperature (diamonds), in comparison with the standard behavior
of Josephson junctions with insulating barriers.

**3 Conductance measurements**

*Measurements of IV curves as a function of temperature highlighted an anomalous IC(T)*
behavior for junctions with barrier thicknesses above 3 nm, which has been extensively
dis-cussed in [7]. In that work, the relevance of the magnetic activity of the barrier is disdis-cussed,
*and a phenomenological model to describe the anomalous IC(T) curves is detailed. Here we*
present measured dI/dV curves and their relation with the presence of triplet coupling inside
the barrier.

In Fig. 2 (a), (e) and (f) are shown the conductance spectra for three junctions with
different spin filter efficiencies (<20%, 97% and 99%) for two different temperatures. For
*all the samples we observe the appearance of two symmetric structures at V ≈ ∆ at low*
temperatures. Similar structures are observed in the presence of a Zeeman splitting that shifts
the spin bands of the superconductor [11]. Since the subgap structures become increasingly
pronounced as the spin polarization increases, it is reasonable to assume for our samples
that these are due to the exchange field induced in the superconducting electrodes by the
GdN barrier. Furthermore, analogous experiments in NbN/GdN/TiN (where TiN is a
non-superconducting metal) do not show any sign of subgap structures, while they show evidence
of an exchange field induced in the NbN superconducting electrode [12]. This implies that the
structures observed in NbN/GdN/NbN Josephson junctions should be related to the exchange
fields induced by GdN in each of the superconducting electrodes.

In addition, we observe a zero-bias peak starting at 4 K up to 10 K [see Fig. 2 (b), (f) and
(j)], and a finite conductance at zero voltage at all temperatures, in contrast with the typical
behavior of a standard BCS junction. Similar features have been reported in NbN/GdN/TiN
junctions, where the zero-bias peak has been related to the presence of odd-frequency
su-perconducting order [13]. However, since the TiN layer is metallic, the Josephson coupling
does not occur and consequently no triplet supercurrent can be observed. In these junctions
the zero-bias peak corresponds to the situation where the superconducting density of states
(DOS) is enhanced at the Fermi level. Similarly, in NbN/GdN/NbN Josephson junctions, the
zero-bias peak should correspond to an unconventional behavior of the DOS of the
super-conducting electrodes in the vicinity of the Fermi level. In order to account for the presence
of available states at the Fermi level, one can use the following modified expression for the
density of states:
ρ(E) = 1
*c + 1*
*Re*
*|E − iΓ|*
*(E − iΓ)*2_{− ∆}
* + c*
(1)

The fitting parameter Γ accounts for the finite lifetime of the Cooper pairs [14] and it has
been used in plenty of experiments to explain the deviation of the measured curves from
the standard exponential subgap of BCS superconductors [15]. As the spin-filter efficiency
increases, we find that the subgap region dI/dV curves becomes almost polynomial instead,
a feature that is reproduced in the simulations by increasing the smearing Γ, thus making it
possible to correlate the shape of the dI/dV curve with the increasing magnetic activity of
the samples. In analogy with the results on NbN/GdN/TiN junctions we include the second
*fitting term c, since Γ alone is not sufficient to account for the finite background conductance*
observed experimentally [12, 13]. The conductance formula can be then obtained deriving
the following expression for the quasiparticle Josephson current [16–18]:

*I ∝ a*
+∞
−∞ ρ1*(E + h)ρ*2*(E − h + V) f(E) − f(E + V) +*
*b*
+∞
−∞
ρ1*(E − h)ρ*2*(E + h + V) f (E) − f (E + V)* (2)
where ρ1and ρ2*are the DOS in the two superconducting electrodes, f (E) is the Fermi *
*func-tion, a and b are coefficient used to model spin filter efficiency and h is the exchange field of*
*the ferromagnet. The coefficient a is the spin filter efficiency, estimated from R(T) curves,*
*while b is chosen so that a + b = 1.*

*As we stated before, the exchange field h is known to cause the Zeeman splitting of the*
spin bands in the superconductor, and the appearance of characteristic subgap features in
dI/dV curves of superconductor/insulator/normal metal junctions. However, in the case of
very high spin polarization one of the two bands is almost completely suppressed, and thus

In Fig. 2 (a), (e) and (f) are shown the conductance spectra for three junctions with
different spin filter efficiencies (<20%, 97% and 99%) for two different temperatures. For
*all the samples we observe the appearance of two symmetric structures at V ≈ ∆ at low*
temperatures. Similar structures are observed in the presence of a Zeeman splitting that shifts
the spin bands of the superconductor [11]. Since the subgap structures become increasingly
pronounced as the spin polarization increases, it is reasonable to assume for our samples
that these are due to the exchange field induced in the superconducting electrodes by the
GdN barrier. Furthermore, analogous experiments in NbN/GdN/TiN (where TiN is a
non-superconducting metal) do not show any sign of subgap structures, while they show evidence
of an exchange field induced in the NbN superconducting electrode [12]. This implies that the
structures observed in NbN/GdN/NbN Josephson junctions should be related to the exchange
fields induced by GdN in each of the superconducting electrodes.

In addition, we observe a zero-bias peak starting at 4 K up to 10 K [see Fig. 2 (b), (f) and
(j)], and a finite conductance at zero voltage at all temperatures, in contrast with the typical
behavior of a standard BCS junction. Similar features have been reported in NbN/GdN/TiN
junctions, where the zero-bias peak has been related to the presence of odd-frequency
su-perconducting order [13]. However, since the TiN layer is metallic, the Josephson coupling
does not occur and consequently no triplet supercurrent can be observed. In these junctions
the zero-bias peak corresponds to the situation where the superconducting density of states
(DOS) is enhanced at the Fermi level. Similarly, in NbN/GdN/NbN Josephson junctions, the
zero-bias peak should correspond to an unconventional behavior of the DOS of the
super-conducting electrodes in the vicinity of the Fermi level. In order to account for the presence
of available states at the Fermi level, one can use the following modified expression for the
density of states:
ρ(E) = 1
*c + 1*
*Re*
*|E − iΓ|*
*(E − iΓ)*2_{− ∆}
* + c*
(1)

The fitting parameter Γ accounts for the finite lifetime of the Cooper pairs [14] and it has
been used in plenty of experiments to explain the deviation of the measured curves from
the standard exponential subgap of BCS superconductors [15]. As the spin-filter efficiency
increases, we find that the subgap region dI/dV curves becomes almost polynomial instead,
a feature that is reproduced in the simulations by increasing the smearing Γ, thus making it
possible to correlate the shape of the dI/dV curve with the increasing magnetic activity of
the samples. In analogy with the results on NbN/GdN/TiN junctions we include the second
*fitting term c, since Γ alone is not sufficient to account for the finite background conductance*
observed experimentally [12, 13]. The conductance formula can be then obtained deriving
the following expression for the quasiparticle Josephson current [16–18]:

*I ∝ a*
+∞
−∞ ρ1*(E + h)ρ*2*(E − h + V) f(E) − f(E + V) +*
*b*
+∞
−∞
ρ1*(E − h)ρ*2*(E + h + V) f (E) − f (E + V)* (2)
where ρ1and ρ2*are the DOS in the two superconducting electrodes, f (E) is the Fermi *
*func-tion, a and b are coefficient used to model spin filter efficiency and h is the exchange field of*
*the ferromagnet. The coefficient a is the spin filter efficiency, estimated from R(T) curves,*
*while b is chosen so that a + b = 1.*

*As we stated before, the exchange field h is known to cause the Zeeman splitting of the*
spin bands in the superconductor, and the appearance of characteristic subgap features in
dI/dV curves of superconductor/insulator/normal metal junctions. However, in the case of
very high spin polarization one of the two bands is almost completely suppressed, and thus

the main signature of the Zeeman splitting in dI/dV curves is a voltage shift corresponding
to the actual exchange energy induced in the superconductor, as observed in NbN/GdN/TiN
*junctions [12, 13]. In order to estimate h, we analyzed the symmetry of the conductance*
spectra of samples with different barrier thicknesses. In Fig. 2 (d), (h) and (l), the positive
and negative branch of the differential conductance are superimposed. For the junction with
lowest spin filter efficiency the two branches overlap, indicating the absence of a significant
exchange field. Assuming an exchange energy with the same magnitude but opposite sign in
the two electrodes, the difference between the positive and negative peaks of the conductance
*is proportional to h.*

*The magnetic field corresponding to the exchange energy h is given by:*

µ0*H =* *2eh*_{gµB} (3)

where µ0*is the vacuum permittivity, e is the electron charge, g is the Lande factor, which is 2*
for GdN, and µBis the Bohr magneton. For the junctions shown in Fig. 2 (h) and (l) the values
obtained for the exchange field are respectively µ0*H = 0.43 ± 0.2T and µ*0*H = −0.17 ± 0.1T.*
These values are far larger than the typical values of the Fraunhofer modulation in these
junctions. The sign of the exchange field is inverted between the two junctions with high
spin polarization and the absolute value decreases with increasing barrier thickness. This
last result is in agreement with previous observations of a decreasing barrier height with
increasing GdN thickness, due to the presence of two Schottky barriers at the interfaces,
*rather than a conventional square barrier, while the sign inversion of the exchange field H*
can be attributed to the changes in the unsaturated GdN domain structure occurring at larger
thicknesses [19].

The fitting curves in Fig. 2 show that Eq. 2 reproduces the experimental data with good
approximation, thus supporting the hypothesis of an unconventional DOS at the Fermi level
related to the exchange fields induced in the superconducting electrodes. In junctions with
high spin polarization, Eq. 2 describing the quasi-particle current gives a very rough
repro-duction of the measured dI/dV curve. This result can be compared with the one reported in
*[7], where the IC(T) behavior can be only roughly reproduced without considering a much*
more complex magnetic structure of the barrier, including a strong asymmetry in the induced
exchange fields. These experimental indications of an increasing asymmetry in the exchange
*fields induced in the NbN electrodes coming from both dI/dV measurements and IC(T) curves*
[Fig. 2 (c), (g) and (k)] are compatible with the presence of spin-triplet transport mechanisms
contributing to the total supercurrent in spin-filter Josephson junctions.

**4 Conclusion**

*The previous observations of anomalous IC(T) curves for high spin filter efficiencies imply*
the presence of spin-triplet supercurrents in NbN/GdN/NbN Josephson junctions. The subgap
structures and the zero bias peak observed in the conductance spectra analyzed in this work
are attributed to an asymmetric induced exchange field in the superconducting electrodes and
to a finite background conductance caused by a non-conventional density of states in the
superconducting electrodes compatible with equal-spin Cooper pairs contributing to the total
current.

**References**

[1] S. Kawabata, S. Kashiwaya, Y. Asano, T. Tanaka, and A. A. Golubov, Phys. Rev. B74, 180502 (2006).

[2] S. Kawabata, Y. Asano, T. Tanaka, A. A. Golubov, and S. Kashiwaya, Phys. Rev. Lett. 104, 117002 (2010).

[3] M. Fogelstrom, Phys. Rev. B62, 11812-11819 (2000).

[4] K. Senapati, M. G. Blamire, Z. H. Barber, Nature Materials10, 849-852 (2012). [5] A. Pal, Z. H. Barber, J. W. A. Robinson and M. G. Blamire, Nature Communications5,

3340 (2014).

[6] D. Massarotti, A. Pal, G. Rotoli, L. Longobardi, M. G. Blamire and F. Tafuri, Nature Communications6, 7376 (2015).

[7] R. Caruso, D. Massarotti, G. Campagnano, A. Pal, H. G. Ahmad, P. Lucignano, M. Eschrig, M. G. Blamire and F. Tafuri, Phys. Rev. Lett.122, 047002 (2019).

[8] L. Longobardi, D. Massarotti, G. Rotoli, D. Stornaiuolo, G. Papari, A. Kawakami, G. P. Pepe, A. Barone and F. Tafuri, Appl. Phys. Lett.99, 062510 (2011).

[9] D. Stornaiuolo, G. Rotoli, D. Massarotti, F. Carillo, L. Longobardi, F. Beltram, and F. Tafuri, Phys. Rev. B87, 134517 (2013).

[10] D. Stornaiuolo, D. Massarotti, R. Di Capua, P. Lucignano, G. P. Pepe, M. Salluzzo, and F. Tafuri, Phys. Rev. B95, 140502 (2017).

[11] R. Meservey, P. Tedrow, and P. Fulde, Phys. Rev. Lett.25, 1270 (1970). [12] A. Pal and M. G. Blamire, Phys. Rev. B92, 180510(R) (2015)

[13] A. Pal, J. A. Ouassou, M.Eschrig, J. Linder and M. G. Blamire, Scientific Reports7, 40604 (2016).

[14] R. C. Dynes, V. Narayanamurti, and J. P. Garno, Phys. Rev. Lett.41, 1509 (1978).
*[15] E. L. Wolf, Principles of Electron tunneling spectroscopy (Oxford University Press,*

Oxford, 2nd edition, 2011)

[16] R. Meservey and P. M. Tedrow, Phys. Rev. B11, 4224-4236 (1975). [17] X. Hao, J. S. Moodera, R. Meservey, Phys. Rev. B42 8235-8244 (1990).

[18] P. M. Tedrow, J. E. Tkaczyk and A. Kumar, Phys. Rev. Lett.56, 1746-1749 (1986). [19] A. Pal, K. Senapati, Z. H. Barber, and M. G. Blamire, Adv. Mater. 25, 5581-5585